3. EFFECTS OF CALCIUM CHLORIDE ON HYDRATION AND PROPERTIES OF CAO-
Table 3.1 presents the chemical and oxide compositions of raw materials (i.e., GGFBS and fly ash), measured using X-ray fluorescence (XRF) (S8 Tiger wavelength dispersive WDXRF spectrometer, Bruker, Billerica, MA, USA), with their loss of ignition (LOI), estimated using TG (SDT Q600, TA Instruments, New Castle, DE, USA). Analytical grades of calcium chloride (Duksan Chemicals, Korea) and calcium oxide (Daejung Chemicals, Korea) were used as activators.
Table 3.1 Chemical compositions of raw materials
GGBFS Fly ash
Oxide (wt%) Oxide (wt%)
CaO 44.24 SiO2 52.26
SiO2 34.30 Al2O3 22.59
Al2O3 14.28 Fe2O3 9.06
MgO 3.26 CaO 6.21
SO3 1.40 MgO 1.82
TiO2 0.71 K2O 1.79
K2O 0.64 Na2O 1.78
Fe2O3 0.54 TiO2 1.27
Na2O 0.27 P2O5 1.21
MnO 0.25 SO3 1.21
SrO 0.07 SrO 0.34
ZrO2 0.03 BaO 0.24
Y2O3 0.01 MnO 0.07
Particle size distributions (See Figure 3.1) of raw materials were measured using a laser diffraction particle-size analyzer (HELOS (HI199) and RODOS, Sympatec, Germany). The size distribution of GGBFS was similar to distributions in the literature [16, 45, 49], but fly ash had relatively larger particles of over 80 μm.
Figure 3.1 Particle size distributions of raw materials
Figure 3.2 presents the XRD patterns of fly ash, GGBFS, and their mixed raw material (74.65%
GGBFS and 20.00% fly ash), which were obtained using a high-power X-ray diffractometer (D/MAX2500V/PC, Rigaku, Japan) with Cu-Kα radiation (λ = 1.5418Å). The XRD patterns were analyzed using X’pert HighScore Plus software  with the International Center for Diffraction Data (ICDD) PDF-2 database  and the Inorganic Crystal Structure Database (ICSD)  . Identified crystalline phases were quartz, mullite, and magnetite in fly ash, and akermanite in GGFBS. Amorphous humps were found in all materials. Particularly, the mixed raw material had a similar amorphous hump from GGBFS, because a relatively small fraction of fly ash was included in the mixed raw material, and the intensity of the amorphous hump of fly ash generally appeared much smaller than that of GGBFS in XRD.
0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1
0.1 1 10 100 1000
Particle size (µm)
Fly ash GGBFS
Figure 3.2 XRD patterns of mixed raw material, fly ash, and GGBFS. The numbers in parentheses are ICDD PDF-2 or ICSD data numbers for identified phases
All the mixture proportions shared the fixed weight proportion of 40% CAS binder, 40%
GGBFS, and 20% fly ash (i.e., these components constitute CAS 4:4:2) to replicate the proportion among raw materials in PC 4:4:2, as shown in Table 3.2. Every CAS binder in each sample in Table 3.2 had a fixed ratio of 1:9 between CaO and GGBFS, but the samples, denoted 0CSF, 1CSF, 2CSF, and 3CSF, contained different percentages of CaCl2 of 0%, 1%, 2%, and 3%, respectively, to the total weight of CAS 4:4:2. The numbers behind the hyphens in the sample labels indicate water-to-binder (w/b) ratios.
It should be noted that two GGBFSs are seen in separate spaces in each row of Table 3.2, even though all the GGBFSs in this study were obtained from the same supply of GGBFS. Although this may lead to confusion in the readers’ understanding, the notation of two separate GGBFSs was necessary to imitate a ternary blended mixture. Accordingly, the actual total contents in wt% of GGBFS in 0CSF, 1CSF, 2CSF, and 3CSF were 76.0, 75.1, 74.2, and 73.3, respectively. In addition, to investigate the effect of the w/b, three different ratios (w/b = 0.30, 0.35, and 0.40) were used.
Freshly mixed pastes were cast in cubic molds (5×5×5cm) for compressive strength testing.
Cylindrical samples (ϕ2.54×2.54cm) were also prepared for MIP and SEM tests. The cast paste samples
Magnetite (98-015-8743) Quartz (98-015-6196)
Mulite (98-002-3726) GGBFS
Position [°2Theta] (Copper (Cu))
10 20 30 40 50 60
Akermanite (98-002-6683) Fly ash Mixed raw material :
74.65% of GGBFS
& 20.00% of Fly ash Amorphous hump
were manually compacted to remove entrapped air voids, and they were demolded after 24 h. All the samples were cured at a constant temperature of 23 °C and at 99% humidity for 3, 7 and 28 days. After compressive strength tests, the fractured samples were gathered and were finely ground for TG and XRD measurements. Then hydration was stopped using solvent exchange with acetone  with vacuum drying.
Table 3.2 Mixture proportions (wt%)
Group Sample label
CAS (A) GGBFS w/b
Fly ash (C)
Sum (A+B+C) CaCl2 CaO GGBFS Sum
0CSF-0.30 0.0 4.0 36.0 40.0 40.0 20.0 100.0
1CSF-0.30 1.0 3.9 35.1 40.0 40.0 20.0 100.0
2CSF-0.30 2.0 3.8 34.2 40.0 40.0 20.0 100.0
3CSF-0.30 3.0 3.7 33.3 40.0 40.0 20.0 100.0
0CSF-0.35 0.0 4.0 36.0 40.0 40.0 20.0 100.0
1CSF-0.35 1.0 3.9 35.1 40.0 40.0 20.0 100.0
2CSF-0.35 2.0 3.8 34.2 40.0 40.0 20.0 100.0
3CSF-0.35 3.0 3.7 33.3 40.0 40.0 20.0 100.0
0CSF-0.40 0.0 4.0 36.0 40.0 40.0 20.0 100.0
1CSF-0.40 1.0 3.9 35.1 40.0 40.0 20.0 100.0
2CSF-0.40 2.0 3.8 34.2 40.0 40.0 20.0 100.0
3CSF-0.40 3.0 3.7 33.3 40.0 40.0 20.0 100.0
As the presence of CaCl2 in the mixtures might produce an excessive heat of reaction.
Isothermal calorimetry was conducted to measure the hydration kinetics of CAS 4:4:2. The hydration heat of CAS 4:4:2 was examined for the samples with w/b = 0.3 (i.e., samples in Group 1) using the three-point multipurpose conduction calorimeter (Tokyo-Riko Co., Ltd., Japan) for the first 72 h at an initial operation temperature of 25 °C. To compare the heat generation with that of PC, the hydration heat of PC was also measured using the same instrument. In this study, PC was selected for testing rather than PC 4:4:2, because a comparison with the hydration heat of PC is more easily understandable for readers.
Powder XRD patterns were recorded for hardened samples from Groups 1 and 3 using a high- power X-ray diffractometer (D/MAX2500V/PC, Rigaku, Japan) with Cu-Kα radiation (λ = 1.5418Å) within a range of 5 to 60°. All the XRD patterns were analyzed using X’pert HighScore Plus software with the International Center for Diffraction Data (ICDD) PDF-2 database and the Inorganic Crystal Structure Database (ICSD).
TG measurements were performed to analyze the reaction products of each mixture in Groups 1 and 3 using a simultaneous thermal analyzer (SDT Q600, TA Instruments, USA) with a heating rate of 30 °C/min from 30 to 1,010 °C in a nitrogen atmosphere in an alumina pan.
To measure the pore-size distribution of each mixture in Groups 1 and 3, MIP (Auto pore IV, Micrometrics, USA) was used. To increase the reliability of the test results, five identical cubic MIP samples for each mixture proportion were prepared and tested. A sample volume of 125 mm3 (5 mm × 5 mm × 5 mm) was used, and it was kept immersed in isopropanol to cease any further hydration before the testing day.
At 28 days, microstructures of hardened samples were observed on the samples from Group 1, using a high-resolution field emission SEM (S-4800, Hitachi, Tokyo, Japan) with energy dispersive X- ray spectroscopy (EDS). To this end, specimens with a thickness of 2 mm along the length of the cylindrical samples were made using a precision saw. The sliced specimens were immersed in isopropanol to stop hydration. Back-scattered electron (BSE) images and element compositions were obtained from polished surfaces of the sliced samples, prepared using a grinder-polisher (EcoMet 250, Buehler, USA) with a final grit of 1/4 µm of diamond polishing compounds.
Since, in the presence of CaCl2, steel corrosion may be a serious problem when CAS 4:4:2 binders are applied to reinforced concrete structures, electrical resistivity was measured to evaluate the possibility of steel corrosion using Wenner four-probe electrical resistivity measurements .
According to KS L ISO 679 , CAS 4:4:2 binders (i.e., 0CSF, 1CSF, 2CSF, and 3CSF) were prepared with prismatic mortars (binder-to-sand weight ratio = 1:3). Here, an increased w/b ratio (i.e., 0.5) was used in accordance with KS standard requirements. Figure 3.3 describes the prismatic sample with dimensions of 20.0×20.0×17.5cm with a single reinforcing steel bar (rebar) embedded in the center. To prevent any possible corrosion on the exposed surfaces of each rebar, its two end surfaces were sealed using epoxy . The electrical resistivity measurements of the hardened samples were taken at 3, 7, 14, 21, 28, and 56 days. Wenner array probes were placed on the top (plane 1) and side (plane 2) surfaces.
Figure 3.3 Measuring electrical resistivity of the mortar samples (sand-to-binder ratio = 1:3 at w/b = 0.5): (a) prismatic sample and (b) front and back views of the prismatic sample